Strain gradient plasticity modeling of the cyclic behavior ... crystal plasticity as demonstrated...
Embed Size (px)
Transcript of Strain gradient plasticity modeling of the cyclic behavior ... crystal plasticity as demonstrated...
Contents lists available at ScienceDirect
Journal of the Mechanics and Physics of Solids
Journal of the Mechanics and Physics of Solids 79 (2015) 1–20
journal homepage: www.elsevier.com/locate/jmps
Strain gradient plasticity modeling of the cyclic behavior of laminate microstructures
Stephan Wulfinghoff a,n, Samuel Forest b, Thomas Böhlke a
a Karlsruhe Institute of Technology (KIT), Institute of Engineering Mechanics (Continuum Mechanics), Kaiserstraße 12, 76131 Karlsruhe, Germany b Mines ParisTech, Centre des Matériaux, CNRS UMR 7633 BP 87, 91003 Evry Cedex, France
a r t i c l e i n f o
Article history: Received 24 September 2014 Received in revised form 17 December 2014 Accepted 9 February 2015 Available online 11 March 2015
Keywords: Gradient plasticity Non-smooth defect energy Sub-differential Regularization Logarithmic defect energy
x.doi.org/10.1016/j.jmps.2015.02.008 96/& 2015 Elsevier Ltd. All rights reserved.
a b s t r a c t
Two recently proposed Helmholtz free energy potentials including the full dislocation density tensor as an argument within the framework of strain gradient plasticity are used to predict the cyclic elastoplastic response of periodic laminate microstructures. First, a rank-one defect energy is considered, allowing for a size-effect on the overall yield strength of micro-heterogeneous materials. As a second candidate, a logarithmic defect energy is investigated, which is motivated by the work of Groma et al. (2003). The properties of the back-stress arising from both energies are investigated in the case of a laminate microstructure for which analytical as well as numerical solutions are derived. In this context, a new regularization technique for the numerical treatment of the rank-one potential is presented based on an incremental potential involving Lagrange multipliers. The results illustrate the effect of the two energies on the macroscopic size-dependent stress–strain response in monotonic and cyclic shear loading, as well as the arising pile-up distributions. Under cyclic loading, stress–strain hysteresis loops with inflections are predicted by both models. The logarithmic potential is shown to provide a continuum formulation of Asaro's type III kinematic hardening model. Experimental evidence in the literature of such loops with inflections in two-phased FFC alloys is provided, showing that the proposed strain gradient models reflect the occurrence of reversible plasticity phenomena under reverse loading.
& 2015 Elsevier Ltd. All rights reserved.
Many industrial projects require systematic and efficient methods in order to miniaturize systems and design new material micro-structures successfully. Therefore, there is an increasing need for micro-mechanical material models. In this context, size effects are of particular importance. These are not captured by classical plasticity theories which do not possess an internal length scale.
This deficiency has motivated the mechanical community to enhance the classical constitutive equations. In particular, additional microstructural information is taken into account. In most cases, the kinematical framework is extended by plastic strain gradients. This choice is motivated by the correlation between size effects and plastic inhomogeneity, ex- perimentally observed and predicted by dislocation mechanics (Hall, 1951; Petch, 1953; Stölken and Evans, 1998; Xiang and Vlassak, 2006; Gruber et al., 2008; Groma et al., 2003; Mesarovic et al., 2010, 2015).
www.sciencedirect.com/science/journal/00225096 www.elsevier.com/locate/jmps http://dx.doi.org/10.1016/j.jmps.2015.02.008 http://dx.doi.org/10.1016/j.jmps.2015.02.008 http://dx.doi.org/10.1016/j.jmps.2015.02.008 http://crossmark.crossref.org/dialog/?doi=10.1016/j.jmps.2015.02.008&domain=pdf http://crossmark.crossref.org/dialog/?doi=10.1016/j.jmps.2015.02.008&domain=pdf http://crossmark.crossref.org/dialog/?doi=10.1016/j.jmps.2015.02.008&domain=pdf http://dx.doi.org/10.1016/j.jmps.2015.02.008
S. Wulfinghoff et al. / J. Mech. Phys. Solids 79 (2015) 1–202
Plastic deformation gradients can be interpreted physically because they define geometrically necessary dislocations (GNDs, see Ashby, 1970). GNDs represent the effective (or net) Burgers vector of the underlying dislocation network. In other words, the presence of GNDs is associated with the incompatibility of the mesoscopic plastic distorsion.
Extending the kinematical plasticity framework by GNDs has a major advantage: it renders the introduction of additional field variables obsolete.1 However, the geometrical description of GNDs is not unique. For example, they may be represented by scalar edge and screw densities. These are defined for each slip system and interact through constitutive models (e.g. Gurtin et al., 2007).
Alternatively, the kinematical extension may be based on the full dislocation density tensor (Nye, 1953; Kröner, 1958). In this case, the interaction is implicitly defined (although little is known about the accuracy of this approach). The advantage of this pragmatic approach is to limit the number of additional degrees of freedom introduced in the theory and in its computational treatment. The present contribution is based on formulations involving the full dislocation density tensor because they are amenable to intensive 3D finite element simulations, in contrast to GND density based models which are much more demanding in terms of degrees of freedom and specific interface conditions at grain boundaries. This is a restrictive approach from the physical point of view but it already contains essential physical features of strain gradient crystal plasticity as demonstrated for instance in the works by Cordero et al. (2012) and Wulfinghoff et al. (2013a). However several aspects of the proposed analysis are applicable to GND density based theories. Phenomenological formulations based on the introduction of the dislocation density tensor are known to give rise to a backstress associated with kinematic hardening, as derived from continuum thermodynamics (Steinmann, 1996; Forest, 2008).
The extension of the kinematical framework allows for the desired modification of the constitutive model. Often, new generalized stresses are introduced, which are conjugate to the additional kinematical quantities (i.e. the gradients) in the power of internal forces. This usually implies extra balance equations (and associated boundary conditions) in addition to the linear momentum balance.
The system of equations must be closed by new constitutive bulk and interface models. This may be achieved by modeling the impact of strain gradients on the bulk energy density, for example. Usually, this is related to a backstress, which appears as an additional term in the flow rule.
Physically, the introduction of additional energy density terms may be motivated by the incompleteness of the con- tinuum theory. Clearly, the continuum description does not contain the full information on the discrete dislocation mi- crostructure. In particular, single dislocations are not resolved. Instead, the continuum representation may be interpreted as a smoothed version of the real system, where information is lost deliberately. Clearly, there is no reason to assume that the total elastic energy of the continuum representation coincides with the elastic energy of the real system including discrete dislocations. This is due to the loss of information as a result of the smoothing procedure (Mesarovic et al., 2010). Additional energy terms in gradient plasticity may therefore be interpreted as an attempt to partially compensate the error in the continuum elastic energy. This is done by taking into account available kinematical information on the dislocation micro- structure as additional argument of the energy.
The optimal form of the energy is subject of current research. Typical models often involve internal length scale para- meters. These are normally assumed to be additional material constants (usually without further physical interpretation). Most applications are based on a pragmatic quadratic approach (e.g. Cordero et al., 2012; Reddy et al., 2012; Wulfinghoff and Böhlke, 2012; Miehe et al., 2013 Wulfinghoff et al., 2013a,b).
However, the microstructure of a crystal is essentially determined by dislocations. Consequently, no microstructural feature justifies the internal length scale to be fixed. Instead, a more reasonable approach seems to be based on a variable internal length scale as a function of the dislocation state (Groma et al., 2003; Mesarovic et al., 2010).
The quadratic form was recently shown to provide physically unrealistic scaling in the size-dependent response of la- minate microstructures under shear (Cordero et al., 2010; Forest and Guéninchault, 2013). Since quadratic forms are unusual in classical dislocation theory, alternative free energy potentials were proposed in the past ten years. Rank-one energies that are linear with respect to the GND densities have been shown to lead to a size-dependent yield stress in certain situations. Additionally motivated by line tension (and more elaborate) arguments, they are used by several authors (Ortiz and Repetto, 1999; Conti and Ortiz, 2005; Ohno and Okumura, 2007; Kametani et al., 2012; Hurtado and Ortiz, 2013).
Asymptotic methods can be used to derive alternative effective potentials for distributions of edge dislocations. The asymptotic derivation of a logarithmic potential by De Luca et al. (2012) accounts for line tension effects at the macroscopic scale. Systematic derivations of backstress distributions were derived in Geers et al. (2013)